Why Use Ionic Liquids for Electrodeposition?
Andrew P. Abbott1, Frank Endres2, and Douglas R. Macfarlane3
1University of Leicester, Department of Chemistry, University Road, Leicester LE1 7RH, United Kingdom 2Clausthal University of Technology, Institute of Electrochemistry, Arnold-Sommerfeld-Street 6,
38678 Clausthal-Zellerfeld, Germany
3Monash University, School of Chemistry, Wellington Road Clayton, VIC3800 Australia
At the start of the ﬁrst edition, it seemed pertinent to pose the question “Why use ionic liquids for electrodeposition?” With over 8 years more experience, it is more suitable to ask “What are the limitations of ionic liquids for electrodeposition?” The previous edition highlighted the lack of background information on many ionic liquid systems, and this edition will ﬁll in quite a bit of this.
The growing interest in the topic in the intervening period is evidenced by the number of publications per year. With about 60 papers per year in 2007, it had grown to 200 papers in 2014. The body of literature that needs to be reviewed has trebled, which highlights the activity. This topic has anh-index of 70.
Electroplating has been carried out for over 200 years, and despite elec-troplated goods entering many aspects of manufacturing industry, very little has changed about the physical processes involved in electrodeposition for about 100 years. It was only with the advent of the electronics industry in the middle of the twentieth century that signiﬁcant changes occurred in the hardware and chemistry of the plating solutions . The postwar period saw an increase in gold plating for electronic components and the use of less hazardous plating solutions. This trend has continued with increased control of hazardous materials to the environment. Improved solution composition and power supply technology have also allowed the development of fast and continuous plating of wire, metal strips, semiconductors, and complex substrate geometries.
Many of the technological developments seen in the electronics industry depend on sophisticated electroplating, including the use of exotic metals, and this is one of the drivers for new technology within the electroplating sector. The other main driver is the search for alternative technologies for metals such as chromium, nickel, and cadmium. Anticorrosion and wear-resistant coatings are predominant in the market for electroplating, and environmental directives will evidently limit their usage in the future.
The main metals that are commercially deposited are Cr, Ni, Cu, Au, Ag, Zn, and Cd together with a number of copper- and zinc-based alloys . The Electrodeposition from Ionic Liquids,Second Edition.
Edited by Frank Endres, Andrew Abbott, and Douglas MacFarlane.
© 2017 Wiley-VCH Verlag GmbH & Co. KGaA. Published 2017 by Wiley-VCH Verlag GmbH & Co. KGaA.
whole electroplating sector is based on aqueous solutions. There are some niche markets based on organic solvents such as aluminum, but these are very much exceptions. Metals not included in this list are generally deposited using plasma vapor deposition (PVD) or chemical vapor deposition (CVD) techniques. These methods allow the coating of most substrates (metal, plastic, glass, ceramic, etc.) not only with metals but also with alloys or compounds (oxide, nitride, carbide, etc.), without damaging the environment. Although these techniques are technically interesting, it is regrettable that they always involve high capital investment and it is diﬃcult to prepare thick coatings; thus, they are only applied to high-value niche markets.
Clearly, the key advantages of using aqueous solutions are as follows: ⚬ Cost
⚬ High solubility of electrolytes
⚬ High conductivities resulting in low ohmic losses and good throwing power ⚬ High solubility of metal salts
⚬ High rates of mass transfer.
For these reasons, water will remain the mainstay of the metal plating industry; however, there are also limitations of aqueous solutions including the following: ⚬ Limited potential windows.
⚬ Gas evolution processes can be technically diﬃcult to handle and result in hydrogen embrittlement.
⚬ Passivation of metals can cause diﬃculties with both anodic and cathodic materials.
⚬ Necessity for complexing agents such as cyanide.
⚬ Water used for almost all of the process steps must been treated before discharge.
These prevent aqueous solutions being applied to the deposition of several technically important materials. In addition, probably the most pressing issue facing the electroplating sector is the introduction of legislation such as Registra-tion, EvaluaRegistra-tion, Authorisation and Restriction of Chemical substances (REACH) in the European Union and similar legislations in other countries, which seek to limit metal precursors such as CrO3, Ni(II), and Co(II) salts as well as metals such as cadmium.
The key technological goals include replacement of environmentally toxic metal coatings, deposition of new alloys and semiconductors, and new coating methods for electronegative metals. The main driving force for nonaqueous electrolytes has been the desire to deposit refractory metals such as Ti, Al, and W. These metals are abundant and excellent for corrosion resistance. It is, however, the stability of their oxides that makes these metals diﬃcult to extract from minerals and apply as surface coatings.
There are clearly a range of alternative nonaqueous solutions that could be used for electrodeposition. Ideally, to obtain the properties required for an electrolyte
1.2 Ionic Fluids 3
solution, polar solvent molecules have to be used, and these should preferably be small in molecular weight and volume, in order to obtain the requisite high ﬂuidity. Unfortunately, all polar solvents result from electronegative elements, which by their nature makes them good electron donors. Accordingly, they will strongly coordinate with metal ions, making them diﬃcult to reduce. While a number of metals have been deposited from polar organic solvents, these tend to be more electropositive metals, and the processes oﬀer few advantages over aqueous solutions. Some studies have been conducted using nonpolar organic solvents, predominantly aromatic hydrocarbons, but these suﬀer from the seri-ous disadvantage that the dissolved electrolytes are highly associated and the solutions suﬀer from poor conductivity. The solutions do, however, have wide potential windows, and it has been demonstrated that metals such as aluminum and titanium can be deposited from them. One of the most successful nonaque-ous processes is the SIGAL process developed in the late 1980s for the deposition of aluminum from toluene [2, 3]. The aluminum source is triethyl aluminum, which is pyrophoric, and despite the high ﬂammability of the electrolyte solu-tion, the process has been commercialized and is still the only electrochemical method for the deposition of aluminum. A review of electrochemistry in non-aqueous solutions is given by Izutsu  and Simkaet al..
Clearly, an alternative to molecular solvents is the use of ionic ﬂuids. Ionic materials typically melt at elevated temperatures due to their large lattice energies. High-temperature molten salts have been extensively used for the electrowinning of metals such as Li, Na, Ti, and Al [6–8]. They have wide potential windows, high conductivities, and high solubilities for metal salts; in fact, they have most of the advantages of aqueous solutions and overcome most of their limitations, but clearly, they suﬀer from the major limitation that the operational conditions are diﬃcult to achieve and limit the range of substrates that can be used for deposition.
The alternative to high-temperature molten salts is to use an ionic substance that melts at a low temperature. While this may sound as an oxymoron, it is log-ical to suppose that the melting point of an ionic substance is related to ionic size, since the greater separation between the charges lowers the lattice energy, and if the ions are made large enough, the material will eventually melt under ambient conditions. A signiﬁcant amount of work was carried out in the middle of the twentieth century with the aim of developing lower temperature molten salts. One of the key aims was to develop a lower temperature melt for aluminum deposition, which led to the formation of Li+/K+/AlCl
3eutectics having freezing
points close to 100∘C . The use of quaternary ammonium salts particularly pyridinium and imidazolium salts eventually pushed the freezing point down to ambient conditions. The term “ionic liquids” was coined to diﬀerentiate these lower temperature ionic ﬂuids from their high-temperature analogs, which are composed predominantly of inorganic ions.
The synthesis and properties of a range of ionic liquids are detailed in the following chapter, while the history and chemical properties of these liquids are
covered in well-known reviews [10, 11]. Since the previous edition, numerous applications of ionic liquids have been commercialized. The most well known of these is BASF’s BASIL process . This uses the ionic liquid as a phase transfer catalyst to produce alkoxyphenylphosphines, which are precursors for the synthesis of photoinitiators used in printing inks and wood coatings. The imidazole acts as a proton scavenger in the reaction of phenyl-chlorophosphines with alcohols to produce phosphines. The Dimersol
®process  has also been commercialized and uses a Lewis-acid catalyst for the dimerization of butenes to produce C8oleﬁns, which are usually further hydroformylated giving C9alcohols used in the manufacture of plasticizers.
A review of successes and applications of ionic liquids is out of date almost as soon as it is published, but some areas where some signiﬁcant developments have been made include batteries, supercapacitors, actuators, dye-sensitized solar cells, gas storage, antistatic agents, and cleaning agents. These applications are covered in numerous reviews [14–17]. Advances in the commercialization of electrodeposition are covered later in this book, but it is suﬃcient to say here that some processes have been taken to a scale where hundreds to thousands of amperes have been applied to working electrodes.
What Is an Ionic Liquid?
The recognized deﬁnition of an ionic liquid is “an ionic material that is liquid below 100∘C,” but this leaves signiﬁcant question as to what constitutes an ionic material. Some authors limit the deﬁnition to cations with discrete anions, for example, BF−4 and NO−3. This deﬁnition excludes the original work on chloroa-luminate systems and the considerable work on other eutectic systems and is therefore unsatisfactory. Systems with anionic species formed by complex equi-libria are diﬃcult to categorize as the relative amounts of ionic species depend strongly on the composition of the diﬀerent components.
Ionic liquids have also been separated into ﬁrst- and second-generation liquids, where ﬁrst-generation liquids are those based on eutectics and second-generation liquids have discrete anions . Others have sought to further divide the ﬁrst-generation liquids into diﬀerent types depending on the nature of the Lewis or Brønsted acid, which complexes (see Chapter 3.2) . While there is some dispute as to whether eutectics with Brønsted acids constitute ionic liquids at all, there are others who seek to widen the description of ionic liquids to include materials such as salt hydrates .
In general, the ﬁrst-generation ionic liquids form because the charge on the ions is delocalized, and this gives rise to a reduction in lattice energy. The majority of ionic liquids are described by equilibrium:
cation+anion+complexing agent↔cation+complex anion (1.1) Potentially complex cations could also be formed using species such as cryptands or crown ethers.
1.3 What Is an Ionic Liquid? 5
The confusion arises from the magnitude of the equilibrium constant. For dis-crete anions such as BF−
4 and even ((CF3SO2)2N)−, the equilibrium lies clearly to
the right of Eq. (1.1). For some eutectic-based liquids, the equilibrium constant is also to the right, for example,
But the addition of more Lewis acid produces other anionic species, Cat+Cl−+2AlCl
The use of less Lewis-acidic metals, for example, ZnCl2or SnCl2, will lead to a small amount of Cl−being present in the mixture. The species formed between
the anion and the complexing agent becomes weaker when a Brønsted acid, for example, urea, is used.
Others have claimed that, in the extreme, water can act as a good Brønsted acid and hydrate salts can act as ionic liquids .
2O+ClO−4 ⋅yH2O (1.6)
This idea has recently been extended to include metal salts with complexants such as acetonitrile and MeCN [21, 22].
Metal salts such as AlCl3and ZnCl2have been found to disproportionate to give both anionic and cationic metal-containing species .
These latter ideas are relatively new and point to a wide range of other metal-containing species being possible. They do, however, illustrate that the current deﬁnition of ionic liquids (only ions, m.p.<100∘C) may indeed be precise but, at the same time, not very useful from the perspective of chemical applications.
Ionic liquids with discrete anions have a ﬁxed anion structure, but in the eutectic-based liquids at some composition point, the Lewis or Brønsted acid will be in considerable excess and the system becomes a solution of salt in the acid. A similar scenario also exists with the incorporation of diluents or impurities; hence, we need to deﬁne at what composition an ionic liquid is formed. Similarly, many ionic liquids with discrete anions are hydrophilic, and the absorption of water is found to sometimes have a signiﬁcant eﬀect on the viscosity and conductivity of the liquids [24–26]; at some point, these mixtures become better considered as concentrated aqueous solutions.
It has recently been shown that water mixtures with DESs can in some cases be beneﬁcial for metal deposition, as the presence of water changes speciation and mass transport. Water–ionic liquid mixtures have been shown to be non-homogeneous microemulsions in some cases and so diﬀusion will be complex, depending on the phase behavior of the metal salt. Recent approaches to over-come this diﬃculty have been to classify ionic liquids in terms of their charge
mobility characteristics  and the correlation between the molar conductivity and ﬂuidity of the liquids .
In this book, a broad range of ionic liquids will be assumed, encompassing all of the aforementioned types because in the discipline of electrodeposition, it is the resultant deposit that is important, rather than the means by, or medium from, which it was obtained. As will be seen later, there is also a very ﬁne line between a concentrated electrolyte solution and an ionic liquid containing diluents.
Technological Potential of Ionic Liquids
A series of transition- and main-group-metal-containing ionic liquids have been formulated, and the feasibility of achieving electrodeposition has been demonstrated for the majority of these metals. Figure 1.1 shows the elements in the periodic table that have been deposited using ionic liquids. Details of these systems are given in the subsequent chapters, and concise summaries exist in reviews [19, 29].
While ionic liquids could potentially be used for all electrodeposition pro-cesses, it is quite clear that technically and economically their inﬂuence will be most signiﬁcant in specialist, possibly niche, applications. The most important of these will probably include the following.
1.4.1 Removal of Toxic Reagents
One of the biggest challenges in electroplating will be the need to comply with leg-islation such as REACH, which is attempting to limit the use of hazardous metal precursors in aqueous processes such as CrO3, NiSO4, and CoCl2[30–32]. The ﬁrst of example of a response to this has been scaled up to semiproduction plant scale by OCAS in Belgium [33, 34] (see Chapter 11). Attempts are also being made to substitute strongly acidic solutions for common metal processing systems .
1995 2000 2005 2010 2015 0 50 100 150 200 Publications Year
Figure 1.1 Publications on the topic of electrodeposition using ionic liquids, 1991 to mid-2015 (Web of Science).
1.4 Technological Potential of Ionic Liquids 7
Direct comparison has recently been carried out between nickel deposition in ionic liquids and the commercial electrolyte. It was shown that similar deposi-tion rates could be obtained despite the diﬀerences in viscosity, but improved metal hardness was achieved in the ionic liquid resulting from diﬀerent deposit morphologies .
1.4.2 Water-Sensitive Metals
This is understandably the area that is most interesting as it could enable the deposition of metals that cannot be deposited using aqueous solutions. Initially, aluminum was the main drive, and this is covered in-depth in Chapter 4. This area has been reviewed by El Abedin and Endres  and Alemany et al. . The wide potential windows of some ionic liquids have been used for the deposition of several other reactive metals including magnesium  and group I metals [40, 41]. Other metals, which are diﬃcult to deposit from molecular solvents, have recently been deposited, for example, Ta and Ru using a variety of pyrrolidinium and imidazolium salts [42–44].
A key advantage of using ionic liquids for this task is that redox potentials can change with metal speciation and can thus be adjusted to the requirements of a particular deposition process. This allows metals that would have disparate redox potentials in aqueous solutions to be codeposited in ionic media. Recent addi-tions to this ﬁeld include the study of Al–Zn , Ti–Al , Al–Mn , and Al–Li  alloys.
1.4.3 Deposition on Water-Sensitive Substrates
Several groups have studied the deposition of metals onto water-sensitive sub-strates, for example, zinc onto magnesium  and aluminum on to magnesium alloys .
1.4.4 Semiconductor Electrodeposition
The deposition of well-characterized semiconductors is an important techno-logical goal. In a similar manner to that practiced with water-sensitive metals, electroplating systems have been developed for a variety of p-block elements including most of groups III, IV, and V. Of particular note is the ability to deposit silicon, germanium, gallium, and indium [51–53] and their alloys such as SixGe1−x
, Bi–Te, Sb–Te , CdTe , and CdS . Ternary and quaternary sys-tems, for example, AlInSb  and Cu2ZnSnS4, have also been produced . The topic of semiconductor deposition is covered in Chapter 6.
1.4.5 Deposition of Nanoarchitectures
In aqueous solutions, metals tend to deposit with a macrocrystalline morphology, whereas in ionic liquids, crystallites for many metals are orders of magnitude smaller. The exact cause of this is not fully understood, but it was shown that there is a deﬁnite cation eﬀect [60, 61] suggesting that the double-layer structure aﬀects deposit morphology. Many authors have shown the importance of a speciﬁc ionic liquid in controlling the morphology of a metallic deposit . It seems that ionic
liquids with bulky cations, particularly those with aromatic moieties, tend to yield smaller architectures compared to those without aromatic moieties. A variety of nanoscale deposits have been produced with the majority aimed at making catalytic surfaces either for synthesis or for sensors .
Two- and three-dimensional microstructures such as wires and macropores can be electrodeposited on an electrode surface by using a templating mask. This is not unique to ionic liquids, but it does enable a wider range of metals to be used. Three-dimensional ordered macroporous (3DOM) ﬁlms can be created by deposition around ordered polymer spheres, and this has been done for Cu  and Si . Electrodeposition through nanoporous polycarbonate ﬁlms has been carried out to produce silver  and aluminum  nanorods with high aspect ratios (l/d∼80−100). The deposition of structured architectures is covered in more detail in Chapter 8.
In the longer term, specialist ionic liquids will enable technically complex high-added value products to be introduced, for example, semiconductor coatings, special magnetic alloys, nanoparticle composite coatings with special erosion/corrosion properties, and metal foams for energy-storage activated surfaces for self-sterilization purposes (e.g., through photocatalysis).
Also, metals have signiﬁcantly diﬀerent reduction potentials in ionic liquid solutions compared to water. For example, the diﬀerence in reduction potential between the Cr and Pt in ionic liquids may be as little as 100 mV, whereas in aqueous solutions, it is in excess of 2 V. One consequence of this characteristic is that alloy coatings may be prepared more readily and that it should be possible to develop many novel alloy coatings. The ﬁrst comparison between aqueous and ionic liquid redox potentials has now been published .
A fundamental advantage of using ionic liquid electrolytes in electroplating is that, since these are nonaqueous solutions, there is negligible hydrogen evolution during electroplating and the coatings possess the much superior mechanical properties of the pure metal. Hence, essentially, crack-free, more corrosion-resistant deposits are possible. This may allow thinner deposits to be used, thus reducing overall material and power consumption still further.
The electrodeposition of metals from ionic liquids is a novel method for the production of nanocrystalline metals and alloys, because the grain size can be adjusted by varying the electrochemical parameters such as overpotential, cur-rent density, pulse parameters, bath composition, and temperature. Recently, for the ﬁrst time, nanocrystalline electrodeposition of Al, Fe, and Al–Mn alloy has been demonstrated.
1.4.6 Health and Safety
The properties of the new electrolyte media could also provide much higher health and safety standards for employees in the workplace, that is, elimination of hazardous vapors, elimination of highly corrosive acidic/alkaline solutions, and substantially reduced use of toxic chemicals. Current aqueous processing systems have a strongly negative impact on the environment (risk of groundwater contamination, soil pollution), which obliges the treatment of wastewater and the dumping of the ultimate waste in landﬁll. The metal ﬁnishing industry in
1.4 Technological Potential of Ionic Liquids 9
general estimates that at least 15% of turnover is related to the cost of treat-ment for environtreat-mental protection. A signiﬁcant issue for the metal ﬁnishing industry is the introduction of REACH, a European Community Regulation (EC 1907/2006) started in June 2007. It uniﬁed a variety of directives and regulations into a single system to protect human health and the environment. The main aims are to handle chemical substance data through supply chains and regulate the use of chemicals of higher concern. The legislation places the burden to manage chemical risks on industry both during manufacture and at the import/export stage. REACH also provides the European administrators with more powers to restrict usage. Similar legislation has been, or is in the process of being, implemented in other countries. Thus, industries using metal ﬁnishing processes must search for new techniques to achieve these environmental goals. In addition to the growing costs and negative eﬀects on competitiveness, it is a question of survival in the years to come. The technology developed by this project is generic to most metal plating systems and as such should represent a signiﬁcant advancement for the environmental sustainability of the metal ﬁnishing and electronics manufacturing sectors.
Of value from a health and safety point of view, many ionic liquids have insignif-icant vapor pressure (thus odorless), some are nontoxic (and even completely biodegradable), and most are highly conductive.
There are, however, numerous risk elements in the development of processes based on these new liquids:
• Coatings must achieve quality standards and a large amount of process devel-opment is required.
• A life cycle analysis (LCA) and an environmental impact study have only been carried out for a limited number of systems.
• Information of scale-up and integration design of generic prototype systems has been gathered, but it is proprietary information.
• Some applications are at fundamental research stage with associated higher risk, that is, electroless, semiconductor, anodizing, and nanocomposite coatings.
• Process economics have been determined for a limited number of processes, but this again is proprietary information.
• For improved existing products, customer acceptance is likely to be a signiﬁ-cant factor, that is, reluctance to change product speciﬁcations.
Some processes are now reaching a scale of development where these issues have been addressed . One has even reached a scale where>1000 A is applied to the working electrode and the electrolyte has been used for>1 year. Most of the information is still proprietary. This does, however, show that many of the issues with ionic liquid scale-up can be overcome. The potential impact is extremely broad and fundamental in nature, because the research will explore a totally inno-vative approach to metal ﬁnishing technology, which has never been exploited previously. The use of this completely diﬀerent type of solvent/electrolyte system entirely changes the normal behavior of metal ﬁnishing processes seen in tra-ditional aqueous electrolytes, and an extensive range of entirely new processes and products can be expected. Information gained to date from pilot studies
shows that deposit morphology is fundamentally diﬀerent from current aqueous deposits.
There are several physical plating parameters that are diﬀerent in an ionic liquid from those in an aqueous solution.
Ionic liquids have wide liquid regions typically in the range from−40 to 250∘C, which allow more thermodynamic control than is possible in aqueous solutions. This may have potential beneﬁts for the development of new alloys. While most studies have been carried out in the range of 25–50∘C, some recent investiga-tions have shown that operating condiinvestiga-tions at∼100∘C can lead to signiﬁcantly diﬀerent morphologies.
Ionic liquids can be diluted with a range of organic and aqueous solvents, and these signiﬁcantly aﬀect conductivity, viscosity, and metal speciation. Some new data has been obtained, especially with water as a diluent. It has also been found that ionic liquids added to aqueous plating baths can act as brighteners. These eﬀects have been ascribed to double-layer eﬀects and changes in speciation.
1.4.9 Cation and Added Electrolytes
Cationic structure and size will aﬀect the viscosity and conductivity of the liquid and hence will control mass transport of metal ions to the electrode surface. They will also be adsorbed at the electrode surface at the deposition potential; hence, the structure of the double layer is dominated by cations. Some studies have shown that changing the cationic component of the ionic liquid changes the structure from microcrystalline to nanocrystalline (see Chapter 9). While these changes are undeniable, more studies need to be carried out to conﬁrm that it is a double-layer eﬀect. If this is in fact the case, then the potential exists to use the cationic component in the liquid as a built-in brightener. The double layer in ionic liquids is now better understood . Most of the electrode charge is compensated in the ﬁrst layer of counterions, and this is followed by a series of layers of opposite charges. AFM - atomic force microscopy has been used to determine the structure at the electriﬁed interface, and electrolytes such as LiCl have been shown to disrupt this interfacial structure .
1.4.10 Anode Material
In aqueous solutions, the anodic processes are either breakdown of the electrolyte solution (with oxygen evolution at an inert anode being favored) or the use of soluble anodes. The use of soluble anodes is limited by the passivation of many metals in aqueous solutions. In ionic liquids, however, the ﬁrst option is not viable due to the cost and nature of the anodic breakdown products. New strategies will therefore have to be developed to use soluble anodes where possible or add a sacriﬁcial species that is oxidized to give a benign gaseous product.
1.5 Conclusions 11
Brighteners are added to most aqueous electroplating solutions and work by either complexing the metal ions and decreasing the rate of nucleation or by acting as an interfacial adsorbate blocking nucleation and hindering growth. Aqueous brighteners have not been studied in ionic liquids, and it is doubtful that they will function in the same way as they do in water because of the diﬀerence in double-layer structure and mass transport.
A small amount of work has been carried out into brighteners that complex the metal ions in solution (see Chapter 11), but again no systematic studies have been carried out. Brighteners, which rely on electrostatic or hydrophobic inter-actions, may function in ionic liquids, but their eﬃcacy is likely to be surface- and cation/anion-speciﬁc. As with other solutes in ionic liquids, the general rule of “like dissolving like” is applicable, that is, ionic species will generally be soluble as will species capable of interacting with the anion. Aromatic species tend to exhibit poor solubility in ionic liquids consisting of aliphatic cations and vice versa.
Since the ﬁrst edition was published, many of the fundamental issues have begun to be addressed. Researchers have focused on the areas where ionic liquids display a clear advantage over aqueous electrolytes, such as controlling architectures and the deposition of semiconductors. Models of the physical properties are now more developed, and the types of systems that form ionic liquids have been expanded. Aspects such as the activity of brighteners and double-layer structures have now been developed. This topic has become a broad church with a less stringent deﬁnition of what constitutes an ionic liquid. Ionic liquids are now becoming more mainstream, and their success in other application ﬁelds is making their adoption easier. We expect that there will be rather rapid further development in the near future as the technologies become truly practical and the special advantages and outcomes possibly become more widely accepted (Figure 1.2).
Na Li K 1 18 H 2 13 14 15 16 17 He Be B C N O F Ne Mg 3 4 5 6 7 8 9 10 11 12 Al Si P S Cl Ar Ca Sc Ti V Cr Mn Fe Co Ni Cu Zn Ga Ge As Se Br Kr Rb Sr Y Zr Nb Mo Tc Ru Rh Pd Ag Cd In Sn Sb Te I Xe Cs Ba La Hf Ta W Re Os Ir Pt Au Hg Tl Pb Bi Po At Rn Fr Ra Ac Ce Pr Nd Pm Sm Eu Gd Tb Dy Ho Er Tm Yb Lu Th Pa U Np Pu Am Cm Bk Cf Es Fm Md No Lr As metal As alloy As metal and alloy
1 Schlesinger, M. and Paunovic, M. (eds) (2000)Modern Electroplating, 4th edn, John Wiley and Sons, Inc., New York.
2 Peled, E. and Gileadi, E. (1976)Journal of the Electrochemical Society,123, 15–19.
3 Simanavicius, L. (1990)Chemija,3, 3–30.
4 Izutsu, K. (2002)Electrochemistry in Non-aqueous Solutions, Weinheim, Wiley-VCH.
5 Simka, W., Puszczyk, D., and Nawat, G. (2009)Electrochimica Acta,54, 5307–5319.
6 Kruesi, W.H. and Fray, D.J. (1993)Metallurgical Transactions B,24B, 605–615.
7 Fray, D.J. and Chen, G.Z. (2004)Materials Science and Technology,20, 295–300.
8 Grjotheim, C., Krohn, M., Malinovsky, K.M., and Thonstad, J. (1982) Aluminum Electrolysis, 2nd edn, Aluminium-Verlag, Dusseldorf.
9 Lantelme, F., Alexopoulos, H., Chemla, M., and Haas, O. (1988) Electrochim-ica Acta,33, 761–767.
10 Wasserscheid, P. and Welton, T. (2008)Ionic Liquids in Synthesis, 2nd edn, Wiley-VCH Verlag, Weinheim, Germany.
11 Hallett, J.P. and Welton, T. (2011)Chemical Reviews,111, 3508–3576.
12 Maase, M. (2005) inMultiphase Homogeneous Catalysis(eds Cornils and Boy), Wiley-VCH Verlag GmbH and Co. KGaA, Weinheim, Germany, p. 560.
13 Chauvin, Y., Olivier, H., Wyrvalski, C.N., Simon, L.C., de Souza, R., and Dupont, J. (1997)Journal of Catalysis,165, 275–278.
14 Plechkova, N.V. and Seddon, K.R. (2008)Chemical Society Reviews,37, 123–150.
15 MacFarlane, D.R., Tachikawa, N., Forsyth, M., Pringle, J.M., Howlett, P.C., Elliott, G.D., Davis, J.H., Watanabe, M., Simon, P., and Angell, C.A. (2014) Energy & Environmental Science,7, 232–250.
16 Kokorin, A. (ed.) (2011)Ionic Liquids: Applications and Perspectives, InTech Publishing.
17 Werner, S., Haumann, M., and Wasserscheid, P. (2010)Annual Review of Chemical and Biomolecular Engineering,1, 203–230.
18 Chiappe, C. and Pieraccini, D. (2005)Journal of Physical Organic Chemistry,
19 Abbott, A.P. and McKenzie, K.J. (2006)Physical Chemistry Chemical Physics,
20 Xu, W. and Angell, C.A. (2003)Science,299, b422.
21 Schaltin, S., Brooks, N.R., Stappers, L., Van Hecke, K., Van Meervelt, L., Binnemans, K., and Fransaer, J. (2012)Physical Chemistry Chemical Physics,
22 Brooks, N.R., Schaltin, S., Van Hecke, K., Van Meervelt, L., Binnemans, K., and Fransaer, J. (2011)Chemistry – A European Journal,17, 5054–5059.
23 Abood, H.M.A., Abbott, A.P., Ballantyne, A.D., and Ryder, K.S. (2011) Chemical Communications,47, 3523–3525.
24 Billard, I., Mekki, S., Gaillard, C., Hesemann, P., Moutiers, G., Mariet, C., Labet, A., and Buenzli, J.G. (2004)European Journal of Inorganic Chemistry,
25 Jarosik, A., Krajewski, S.R., Lewandowski, A., and Radzimski, P. (2006) Jour-nal of Molecular Liquids,23, 43–50.
26 Widegren, J.A., Saurer, E.M., Marsh, K.N., and Magee, J.W. (2005)The Jour-nal of Chemical Thermodynamics,37, 569–575.
27 Abbott, A. P., Ryder, K. S., Licence, P., and Taylor, A. W., What is an Ionic Liquid? In Ionic Liquids Completely UnCOILed, Plechkova and Seddon Eds, John Wiley and Sons Hoboken, NJ, 2015.
28 Abbott, A.P., Harris, R.C., and Ryder, K.S. (2007)Journal of Physical Chem-istry B,111, 4910–4914.
29 El Abedin, S.Z. and Endres, F. (2006)ChemPhysChem,7, 58–61.
30 Eugenio, S., Rangel, C.M., Vilar, R., and Quaresma, S. (2011)Electrochimica Acta,56, 10347–10352.
31 Abbott, A.P., El Ttaib, K., Ryder, K.S., and Smith, E.L. (2008)Transactions of the Institute of Metal Finishing,86, 234–238.
32 Zhu, Y.L., Kozuma, Y., Katayama, Y., and Miura, T. (2009)Electrochimica Acta,54, 7502–7506.
33 Abbott, A.P., Capper, G., Davies, D.L., and Rasheed, R. (2002) Ionic liquids formed from hydrated metal salts.Chemistry – A European Journal,10, 3769–3774.
34 Smith, E.L., Fullarton, C., Harris, R., Saleem, S., Abbott, A.P., and Ryder, K.S. (2010)Transactions of the Institute of Metal Finishing,88, 285–293.
35 Abbott, A.P., Capper, G., Swain, B., and Wheeler, D. (2005) Electropolish-ing of stainless steel in an ionic liquid.Transactions of the Institute of Metal Finishing,82, 51–55.
36 Abbott, A.P., Barron, J.C., Ryder, K.S., and Smith, E.L. (2009) Electrodeposi-tion of zinc using eutectic based ionic liquids.Transactions of the Institute of Metal Finishing,87, 201–207.
37 El Abedin, S.Z. and Endres, F. (2007) Ionic liquids: the link to high-temperature molten salts?Accounts of Chemical Research,40, 1106–1113.
38 Alemany, A., Malkowsky, I., Vagt, U., Maase, M., and O’Meara, M. (2010) Plating and Surface Finishing,97, 34–37.
39 Cheek, G.T., O’Grady, W.E., El Abedin, S.Z., Moustafa, E.M., and Endres, F. (2007) Studies on the electrodeposition of magnesium in ionic liquids. Journal of the Electrochemical Society,155, D91–D95.
40 Howlett, P.C., Brack, N., Hollenkamp, A.F., Forsyth, M., and MacFarlane, D.R. (2006)Journal of the Electrochemical Society,153, A595–A606.
41 Wibowo, R., Aldous, L., Jacobs, R.M.J., Manan, N.S.A., and Compton, R.G. (2011)Chemical Physics Letters,509, 72–76.
42 Ispas, A., Adolphi, B., Bund, A., and Endres, F. (2010)Physical Chemistry Chemical Physics,12, 1793–1803.
43 Borisenko, N., Ispas, A., Zschippang, E., Liu, Q., El Abedin, S.Z., Bund, A., and Endres, F. (2009)Electrochimica Acta,54, 1519–1528.
44 Raz, O., Cohn, G., Freyland, W., Mann, O., and Ein-Eli, Y. (2009) Electrochimica Acta,54, 6042–6045.
45 Pan, S.J., Tsai, W.T., and Sun, I.W. (2010)Electrochemical and Solid-State Let-ters,13, D69–D71.
46 Pradhan, D., Reddy, R.G., and Lahiri, A. (2009)Metallurgical and Materials Transactions B,40B, 114–122.
47 Chen, J., Xu, B., and Ling, G. (2012)Materials Chemistry and Physics,134, 1067–1071.
48 Hudak, N.S. and Huber, D.L. (2012)Journal of the Electrochemical Society,
49 Bakkar, A. and Neubert, V. (2007)Electrochemistry Communications,9, 2428–2435.
50 Chang, J.K., Chen, S.Y., Tsai, W.T., Deng, M.J., and Sun, I.W. (2007) Electro-chemistry Communications,9, 1602–1606.
51 Borisenko, N., El Abedin, S.Z., and Endres, F. (2006)Journal of Physical Chemistry B,110, 6250–6256.
52 Gasparotto, L.H.S., Borisenko, N., Hoeﬀt, O., Al-Salman, R., Maus-Friedrichs, W., Bocchi, N., El Abedin, S.Z., and Endres, F. (2009)Electrochimica Acta,
53 El Abedin, S.Z., Saad, A.Y., Farag, H.K., Borisenko, N., Liu, Q.X., and Endres, F. (2007)Electrochimica Acta,52, 2746–2754.
54 Al-Salman, R., El Abedin, S.Z., and Endres, F. (2008)Physical Chemistry Chemical Physics,10, 4650–4657.
55 Golgovici, F., Cojocaru, A., Nedelcu, M., and Visan, T. (2009)Chalcogenide Letters,6, 323–333.
56 Dale, P.J., Samantilleke, A.P., Shivagan, D.D., and Peter, L.M. (2007)Thin Solid Films,515, 5751–5754.
57 Izgorodin, A., Winther-Jensen, O., Winther-Jensen, B., and MacFarlane, D.R. (2009)Physical Chemistry Chemical Physics,11, 8532–8537.
58 Tsuda, T. and Hussey, C.L. (2008)Thin Solid Films,516, 6220–6225.
59 Chan, C.P., Lam, H., and Surya, C. (2010)Solar Energy Materials & Solar Cells,94, 207–211.
60 Liu, Q.X., El Abedin, S.Z., and Endres, F. (2008)Journal of the Electrochemi-cal Society,155, D357–D362.
61 El Abedin, S.Z., Moustafa, E.M., Hempelmann, R., Natter, H., and Endres, F. (2006)ChemPhysChem,7, 1535–1543.
62 Eiden, P., Liu, Q., El Abedin, S.Z., Endres, F., and Krossing, I. (2009) Chem-istry – A European Journal,15, 3426–3434.
63 Abbott, A.P., Frisch, G., and Ryder, K.S. (2013)Annual Review of Materials Research,43, 1.1–1.24.
64 El Abedin, S.Z., Prowald, A., and Endres, F. (2012)Electrochemistry Commu-nications,18, 70–73.
65 Liu, X., Zhang, Y., Ge, D., Zhao, J., Li, Y., and Endres, F. (2012)Physical Chemistry Chemical Physics,14, 5100–5105.
66 Kazeminezhad, I., Barnes, A.C., Holbrey, J.D., Seddon, K.R., and Schwarzacher, W. (2007)Applied Physics A,86, 373–375.
67 Pomfret, M.B., Brown, D.J., Epshteyn, A., Purdy, A.P., and Owrutsky, J.C. (2008)Chemistry of Materials,20, 5945–5947.
68 Abbott, A.P., Frisch, G., Gurman, S.J., Hillman, A.R., Hartley, J., Holyoak, F., and Ryder, K.S. (2011)Chemical Communications,47, 10031–10033.
69 Alam, M.T., Islam, M.M., and Ohsaka, T. (2010) inElectrochemical Properties and Applications of Ionic Liquids(eds A.A.J. Torriero and M.J.A. Shiddiky), Nova Science Publishers, Inc., New York.
70 Hayes, R., Webber, G.R., Borisenko, N., Corr, B., Endres, F., and Atkin, R. (2012)Chemical Communications,48, 10246–10248.